Strain-dependent magnetic configurations in manganite-titanate
heterostructures probed with soft X-ray techniques
R.V. Chopdekar1,a, J. Heidler1, C. Piamonteze1, Y. Takamura2, A. Scholl3, S. Rusponi4, H. Brune4, L.J. Heyderman1, and F. Nolting1
1 Paul Scherrer Institut, 5232 Villigen PSI, Switzerland
2 Department of Chemical Engineering and Materials Science, University of California, CA 95616 Davis, USA 3 Advanced Light Source, Lawrence Berkeley National Laboratory, CA 94720 Berkeley, USA
4 Institute of Condensed Matter Physics, ´Ecole Polytechnique F´ed´erale de Lausanne, 1015 Lausanne, Switzerland
Received 31 October 2012 / Received in ﬁnal form 11 February 2013
Published online 3 June 2013 – c EDP Sciences, Societ`a Italiana di Fisica, Springer-Verlag 2013
Abstract. We present a detailed study on the strain-induced magnetic domain structure of a (La,Sr)MnO3
thin ﬁlm epitaxially grown on a BaTiO3substrate through the use of polarization-dependent X-ray photoe-mission electron microscopy and X-ray absorption spectroscopy. Angular-dependent measurements allow us to detect vector magnetization on a single-domain scale, and we relate the strain-induced changes in magnetic anisotropy of the ferromagnetic ﬁlm to the ferroelectric domain structure of the underlying substrate using X-ray magnetic circular and linear dichroism spectro-microscopy. Comparisons to mea-surements on a nearly strain free ﬁlm of (La,Sr)MnO3 grown on a (La,Sr)(Al,Ta)O3 substrate illustrate that the BaTiO3 ferroelectric domain structure imprints speciﬁc domain sizes and wall orientations in the (La,Sr)MnO3/BaTiO3 artiﬁcial multiferroic heterostructure. Furthermore, a change of the BaTiO3 ferroelectric domain structure either with temperature or with applied electric ﬁeld results in a corre-sponding change in the (La,Sr)MnO3 ferromagnetic domain structure, thus showing a possible route to obtain room-temperature electric ﬁeld control of magnetic anisotropy at the nanoscale.
Recent studies of artiﬁcial multiferroic heterostructures consisting of epitaxial ferromagnetic and ferroelectric lay-ers have shown large structural, electronic and magnetic changes in the ferromagnetic layer induced by the fer-roelectric layer, illustrating that such artiﬁcial systems can be a promising route to obtaining room tempera-ture magneto-electric coupling in nanoscale systems . Spinel-structure ferromagnetic thin ﬁlms have commonly been used in such artiﬁcial multiferroics, but they exhibit myriad defects such as anti-phase boundaries at the ﬁlm substrate interface , which can reduce the eﬃcacy of the magneto-electric coupling. To avoid such defects, coupling in (La,Sr)MnO3-BaTiO3 (LSMO-BTO) composite multi-ferroics has been explored as a function of temperature as well as applied magnetic and electric ﬁeld.
It is well-known that epitaxial strain can have a large inﬂuence on the Curie temperature and magnetic anisot-ropy of LSMO thin ﬁlms , thus by using a ferroelec-tric substrate such as BTO, one could try to dynamically
Contribution to the Topical Issue “New Trends in
Magnetism and Magnetic Materials”, edited by Francesca Casoli, Massimo Solzi and Paola Tiberto.
a e-mail: Rajesh.Chopdekar@psi.ch
tune the magnetic properties of LSMO. Indeed, this ma-terial system shows coincident changes in LSMO resistiv-ity, magnetization and lattice parameter at phase transi-tions of the BTO substrate [4,5]. Furthermore, an applied electric ﬁeld across a BTO substrate, which changes the relative populations of a- and c-type ferroelectric do-mains, can induce persistent and sharp changes in LSMO magnetization .
While studies have shown that signiﬁcant magneto-electric coupling is possible in the LSMO-BTO system, such results are spatially averaged over macroscopic dis-tances. Thus, for implementation of such materials at technologically relevant length scales, we need a com-prehensive understanding of artiﬁcial multiferroic prop-erties on the sub-micron length scale (i.e. the length scale of single ferroelectric and ferromagnetic domains). With X-ray photoemission electron microscopy (PEEM), we have shown that an artiﬁcial multiferroic system of a spinel magnetostrictive ﬁlm grown on a perovskite piezoelectric substrate can be studied on the length scale of individual ferroic domains, and that the ferroelectric domain struc-ture can imprint domain strucstruc-tures in the ferrimagnetic phase of the artiﬁcial multiferroic . Additionally, X-ray spectroscopy has been shown to oﬀer great insight into the inﬂuence of epitaxial strain sign and magnitude, as well
A series of 29 nm and 53 nm thick LSMO ﬁlms near the op-timal doping concentration (La0.7Sr0.3MnO3) were grown on (001) oriented (La,Sr)(Al,Ta)O3(LSAT) and (001) ori-ented BTO substrates by pulsed laser deposition. Typi-cal deposition conditions (700 ◦C substrate temperature, 300 mTorr O2 partial pressure, 1 J/cm2 laser ﬂuence) for obtaining low roughness LSMO ﬁlms on (001) SrTiO3 were also found to produce ﬁlms with low roughness on LSAT and BTO substrates. The ﬁlms were cooled to 500 ◦C in 300 mTorr O2, then annealed for 20 min in 0.5 atm O2pressure before cooling to room temperature to reduce the density of oxygen vacancies in the ﬁlm. In order to measure any electric ﬁeld-induced changes in the ﬁlm magnetic domain structure, BTO substrates were me-chanically thinned from the back to approximately 0.2 mm after LSMO deposition, and 5 nm Cr/50 nm Au contacts were placed on the back of the thinned BTO substrates.
X-ray PEEM experiments were performed in 16◦ graz-ing incidence at the surface/interface: microscopy (SIM) beamline  at the Swiss Light Source and in 30◦ grazing incidence at the PEEM3 microscope of the Ad-vanced Light Source. Samples were measured in a de-magnetized state; the demagnetizing protocol is described elsewhere. Room temperature total electron yield spec-troscopy measurements were performed at normal inci-dence (X-ray propagation direction along the sample nor-mal) in a ﬁeld of up to 2 T applied in the sample plane at the X-Treme beamline of the Swiss Light Source . It should be noted that the ﬁeld was tilted out of the sample plane by 8◦ to enhance electron yield. Samples were measured at the Mn L3,2 edges (approximately 642 and 653 eV) using greater than 97% linearly polarized and 97% circularly polarized X-rays in the temperature range of 300 K to 580 K at the SIM beamline micro-scope. Additionally, measurements in the temperature range of 160 K to 300 K were taken at the PEEM3 mi-croscope. X-ray magnetic circular dichroism (XMCD), i.e. the diﬀerence in X-ray absorption between left and right circularly polarized X-rays, was utilized to probe the ferro-magnetic properties of the LSMO ﬁlms, whereas X-ray lin-ear dichroism (XLD) relies on the diﬀerence in absorption between horizontally and vertically polarized X-rays and
was extracted from hard X-ray diﬀraction reciprocal space mapping of the 002 and 303 reﬂections of a 53 nm LSMO ﬁlm on a polydomain BTO substrate. The averaged strain of the ﬁlm is in biaxial tension, but the local strain state depends on the orientation of each BTO ferroelectric do-main at the ﬁlm-substrate interface. In the tetragonal phase of BTO an a-axis ferroelectric domain, whose fer-roelectric moment is in the plane of the substrate along a pseudocubic 100 direction, imposes a uniaxial modu-lation of the strain, whereas a c-axis ferroelectric domain imposes a biaxially symmetric strain.
The strain has a marked impact on the magnetic do-main structure as can be seen in the PEEM images of Figure1. The PEEM XMCD image of the LSMO ﬁlm on LSAT has four levels of contrast, signifying four orienta-tions of ferromagnetic domains, labeled A, B, C, and D, evenly distributed across the ﬁeld of view in Figure 1a. As the level of contrast is proportional to the projection of magnetization along the X-ray propagation direction, we can infer that the LSAT sample has domains pointing along four equivalent 110 in-plane directions. We can conﬁrm the in-plane nature of the domains by perform-ing an azimuthal scan of the sample, which shows that each domain has a contrast reversal upon 180◦rotation of the sample, and the maximum level of contrast is equiv-alent for each set of domains. In comparison, the domain structure of LSMO on BTO in Figure1b is heterogeneous, with some regions showing bright and dark contrast and a central stripe showing a neutral contrast. Across the sam-ple, borders between regions of diﬀerent contrast can be oriented along either100 or 110 families of directions, and in the case of Figure1b, the stripe is oriented along a 110 type direction.
The 3D magnetization proﬁle of a given ﬁeld of view can be extracted from images taken at 3 or more azimuthal sample angles. An example of this vector decomposition for the 29 nm thick LSMO/BTO sample is shown in Fig-ure2, which is obtained by ﬁtting the contrast intensity in a point-by-point manner from 5 images at azimuthal an-gles between 0–180◦, and this analysis reveals that the het-erogeneous contrast of Figure 1b is due to regions whose magnetic easy axes lie along alternating  and  directions. The borders between regions are along a110 type direction, and our previous study has shown that this conﬁguration of ferromagnetic domains is due to the
Fig. 1. Mn L3edge PEEM-XMCD images of demagnetized (a) 53 nm thick LSMO/LSAT and (b) 29 nm thick LSMO/BTO samples. White and black contrast indicates magnetization along the X-ray propagation direction, and this direction is shown by the arrow in the lower right of each image. Gray contrast indicates magnetization oblique to the X-ray prop-agation direction. The ﬁlm on LSAT shows fourfold in-plane anisotropy evenly distributed across the ﬁeld of view, whereas the ﬁlm on BTO shows a 5 micron wide striped modulation of the magnetic contrast.
strain imposed by alternatinga-axis domains in the BTO substrate .
Although the LSMO/LSAT sample is nearly strain-free, there is a linear dichroism present at the surface of the sample due to the reduction of coordination of the Mn environment. Spectro-microscopy in the same ﬁeld of view as Figure 1a at grazing incidence using linearly po-larized light is plotted in Figure 3 with a signiﬁcant lin-ear dichrosim at both the L3 and L2 peaks. Comparison of the linear dichroism spectra for the regions labeled A, B, C, and D in Figure 1a reveals that there is a slight change in the spectra between domains whose magnetiza-tion lies almost completely along the X-ray propagamagnetiza-tion direction and domains whose magnetization is oblique to the X-ray propagation direction (Fig.3b). Taking the dif-ference of these spectra (Fig.3c) highlights the magnetic-only contribution to the linear dichroism. The magnitude of this magnetic linear dichroism at the L2edge is approx-imately 2% of the maximum X-ray absorption signal, and
Fig. 2. Vector decomposition of magnetization along
100-type directions for the 29 nm thick LSMO/BTO sample.
we can estimate that the magnetic contribution is half of the total linear dichroism signal at the L2 edge at room temperature.
We may directly compare the magnetic linear dichro-ism spectrum extracted from the demagnetized spectro-microscopy experiment to a magnetic linear dichroism spectrum measured in applied ﬁeld. In normal incidence geometry, there are equivalent 100 axes that we can probe by aligning the electric ﬁeld component of the lin-early polarized X-rays along either the horizontal or verti-cal directions (e.g.E  or E ). In zero applied magnetic ﬁeld for a demagnetized sample, we would aver-age over all ferromagnetic domains and there would be no net diﬀerence in absorption. However, application of a 2 T magnetic ﬁeld in the plane of the sample along the  direction saturates the LSMO ﬁlm into a single domain state and thus we may probe magnetic-only contribution to the linear dichroism (XMLD). While the XMLD line-shapes for the LSMO/LSAT sample in Figures3and4are similar, comparison of the XMLD spectra for the 53 nm LSMO ﬁlms on LSAT and BTO shown in Figure 4 have qualitatively diﬀerent lineshapes, illustrating that the av-erage tensile strain aﬀects the magnetic anisotropy of the LSMO ﬁlm on BTO as compared to the LSAT sample. As the epitaxial strain state imposes a distortion of the local Mn environment and thus alters the ligand ﬁeld, a diﬀerence in the XMLD spectra can be expected. Indeed, such diﬀerences in ligand ﬁeld due epitaxial strain between LSMO and dielectric substrates has been previously estab-lished (e.g. Ref. ). To demonstrate the dynamic tuning of ﬁlm magnetic properties by modulation of strain state via the ferroelectric substrate, we can manipulate the fer-roelectric domain population with either temperature or applied electric ﬁeld.
Fig. 3. (a) Mn L3 polarization averaged X-ray absorption
spectrum of 53 nm thick LSMO/LSAT sample measured via PEEM spectromicroscopy in grazing incidence. (b) A large lin-ear dichroism from both structural and magnetic origins is present when comparing absorption of X-rays with polariza-tion oriented along in-plane versus out-of-plane direcpolariza-tions, and (c) the magnetic-only dichroism can be measured by taking the diﬀerence of linear dichroism spectra between areas magne-tized along orthogonal in-plane directions (e.g. areas B and D) whereas no diﬀerence in dichroism signal is seen for areas with antiparallel magnetization (e.g. areas C and D).
Fig. 4. Mn L3,2 X-ray magnetic linear dichroism spectra of the 53 nm thick (a) LSMO/LSAT and (b) LSMO/BTO sam-ples measured at normal incidence, comparing X-ray absorp-tion along in-plane  and  direcabsorp-tions with H = 2 T . There are strain-induced diﬀerences between the XMLD spectra, such as an increase in XMLD intensity near 641 eV and 653 eV for the LSMO/BTO sample.
Fig. 5. (a) Images taken in the same area with PEEM-XLD
(left) and XMCD (right) for the 29 nm thick LSMO/BTO sam-ple at room temperature and 375 K. The arrow indicates the X-ray propagation direction. (b) Temperature dependence of XLD and XMCD intensity across the LSMO Curie tempera-ture (T ≈ 350 K) and the BTO tetragonal-cubic phase transi-tion (T ≈ 410 K).
3.2 Temperature-induced changes in magnetic domain structure
Temperature-dependent imaging of the LSMO/BTO sam-ple with XMCD and XLD at the Mn L edges (Fig. 5) show that there is a strong temperature dependence of both XMCD and XLD intensity in the temperature range from 300 K to 450 K. Figure 5a illustrates the spatially resolved change in XMCD and XLD for temperatures below and above the Curie temperature of the LSMO ﬁlm, while Figure 5b plots the maximum diﬀerence in XMCD contrast between white and black domains at the L3 edge peak and diﬀerence in XLD contrast at the L2 edge between the two variants of LSMO on a-axis BTO domains. The XMCD contrast converges to zero at ap-proximately 350 K, close to the bulk Curie temperature of LSMO (370 K). The XLD contrast temperature depen-dence has two steps near 350 K and 425 K, which are near the Curie temperatures of LSMO and BTO, respectively. In the temperature range between 350 K and 425 K, the LSMO ﬁlm is non-magnetic but still experiences the struc-tural distortion imposed by the ferroelectric substrate do-main structure. Thus at room temperature there are both magnetic and structural contributions to the linear dichro-ism, and the persistence of the structural linear dichroism up to the BTO ferroelectric Curie temperature illustrates
Fig. 6. PEEM-XMCD (top) and XLD (bottom) images for
the 53 nm thick LSMO/BTO sample during a cooling cycle going from room temperature to 160 K and back. The circled region indicates the same physical location on the LSMO ﬁlm.
the strong inﬂuence that the BTO domain structure has on the local Mn environment.
Similarly, on cooling to the tetragonal-orthorhombic (T≈ 290 K) and orthorhombic-rhombohedral (T ≈ 190 K) phase transitions of BTO, the BTO domain popu-lation changes and both domain wall motion and a change in easy axis of the LSMO ﬁlm can be seen (Fig. 6). By monitoring the same area of the LSMO ﬁlm during a tem-perature cycle from 300 K to 160 K to 300 K, we can record the evolution of XMCD and XLD as the sample traverses BTO phase transitions. The original magnetic domain conﬁguration was set by demagnetizing the sam-ple, and illustrates the domain conﬁguration in a region strained by a largea-axis BTO domain similar to the re-gions shown in Figure 1b. The sample is measured at a slight angle away from the  direction to measure pro-jections of magnetization along either 100 or 110 di-rections. By geometry, we expect strong contrast for do-mains along the  axis, an intermediate contrast along the  axis, and almost no contrast for domains along either the  in-plane axis or  out-of-plane axis.
Upon traversing each phase transition in zero applied magnetic ﬁeld, the original demagnetized domain struc-ture with LSMO domains signiﬁcantly oriented along the  axis as shown at 297 K changes into a heteroge-neous contrast pattern as shown by the XMCD image at 227 K, and the single a-axis region of BTO changes into a multidomain conﬁguration as shown by the change in linear dichroism domain pattern in the orthorhombic phase. While the original magnetic domain conﬁguration in the circled region had a strong alignment along the  axis, when returning to 296 K the domains in this region have a neutral contrast, showing that the tempera-ture cycling has produced a 90◦rotation of magnetization for these domains due to reconﬁguring the ferroelectric domain structure of the underlying substrate.
The change in XMCD intensity across a single phase transition is plotted in Figure7. By evaluating the change
Fig. 7. PEEM single polarization images of the 53 nm thick
LSMO/BTO sample at the Mn L3 edge at (a) 165 K (rhom-bohedral BTO) and (b) 200 K (orthorhombic BTO), with six example regions selected. The ﬁeld of view is 36 microns. In panel (c), the XMCD intensity is determined for each region, illustrating a change from four contrast levels below 187 K to three contrast levels above 187 K.
in XMCD contrast, equivalent to the projection of the magnetization along the beam direction, we see that the XMCD contrast levels strongly change in individual do-mains from four distinct levels of contrast (fourfold easy axis evenly distributed in the ﬁeld of view) in the BTO rhombohedral phase to three levels of contrast with areas either strongly aligned along the X-ray direction or oblique to the X-ray direction. In other words, in the orthorhom-bic phase we have areas with a uniaxial magnetic easy axis either along or oblique to the X-ray direction. Com-parison to spatially averaged bulk magnetometry measure-ments on LSMO/BTO show that a rotation of magnetic anisotropy from 110 type directions to 100 type di-rections can occur across the BTO phase transition . Thus, a magnetization rotation of either 45◦ or 90◦ can be generated in the LSMO/BTO system by manipulating the ferroelectric phase and orientation of ferroelectric axis with temperature.
3.3 Electric field-induced changes in magnetic domain structure
It is also possible to manipulate the BTO domain popu-lation at a given temperature by application of an electric ﬁeld. In this case, during PEEM imaging we hold the LSMO ﬁlm at ground potential with respect to the sample holder and apply a voltage pulse to the back of the sample, thus we can apply more than 5 kV/cm across the BTO
Fig. 8. Mn L edge XMCD and XLD images for the 29 nm thick
LSMO ﬁlm on BTO before (a, b) and after (c, d) a 10 kV/cm pulse applied across the BTO substrate thickness, with an ar-row indicating the X-ray incidence direction. In this ﬁeld of view, the BTO pre-pulse state has a majority of a-axis do-mains with a 4 micron wide thin stripe ofc-axis domain with domain walls along the in-plane  direction. After the pulse, the change in BTO domain structure as probed with Mn XLD contrast is coincident with rotation of the LSMO magnetiza-tion direcmagnetiza-tion in the thin stripe area. The XMCD contrast scale is the same for panels (a, c) and the XLD contrast scale is the same for panels (b, d).
substrate thickness. Application of a voltage pulse across the thickness of a thermally randomized BTO substrate with both a and c domains (Fig. 8) results in a conver-sion of a-type domains to c-type domains. In Figure8, the XLD domain boundaries before poling are along the  direction, thus the BTO in this region is a majority of a-type domains with a central c-a-type domain stripe . At the boundary between a- and c-type ferroelectric domains, the LSMO domain structure diﬀers in contrast, with the magnetization of the LSMO on the c-axis BTO domain oriented along the X-ray propagation direction and the magnetization of the LSMO on the a-axis BTO domain oblique to the X-ray propagation direction.
gion reversed with the application of the voltage pulse, we could expect inﬂuence of both charge and strain eﬀects on the magnetization of LSMO. While previous studies have shown that an 11 unit cell thick LSMO ﬁlm can demon-strate a signiﬁcant change in properties due to induced charge from an adjacent Pb(Zr,Ti)O3 layer , it is un-clear if such a similar change in interfacial charge would aﬀect a 29 nm thick LSMO ﬁlm. Further work is needed to elucidate the mechanism of this magnetization rotation and the roles that modulation of strain and induced charge play at the LSMO/BTO interface.
In Figure 9, a schematic summarizing the strain-induced magnetic domain conﬁgurations of LSMO due to the ferroelectric domain conﬁguration of BTO is pre-sented. At room temperature, LSMO coupled to ana-axis BTO domain (Fig.9a) exhibits a uniaxial strain state and a strong in-plane uniaxial magnetic anisotropy, whereas LSMO coupled toc-axis BTO (Fig.9b) has a biaxial strain state and weak fourfold in-plane anisotropy. Above 350 K, LSMO is paramagnetic (Fig. 9c) but a structural dis-tortion in LSMO induced by the BTO is still present. Above 425 K, BTO is paraelectric (Fig.9d) and the LSMO XLD intensity induced by the BTO ferroelectric domain structure vanishes. For comparison, the dominant contri-bution to XLD for LSMO grown on LSAT (Fig. 9e) is due to ferromagnetic ordering. As shown experimentally in Figure8and schematically in Figure9, we have demon-strated that by rotating the ferroelectric axis in the BTO substrate with an electric ﬁeld pulse, we have reoriented the magnetization of the LSMO due to the strong elastic interaction between the ﬁlm and substrate.
We have resolved the strain-dependent eﬀect of BTO fer-roelectric domains on LSMO magnetic domains, and have measured the temperature dependence of the magnetic anisotropy of LSMO across the BTO phase transitions. There is a strong eﬀect on the LSMO easy axis due to modulation of strain bya-axis BTO domains, namely an LSMO easy axis rotation of 45◦ when going from the rhombohedral to the orthorhombic BTO phase, and we have measured the eﬀect of reorientation of these BTO do-mains at the spatial resolution of a single LSMO domain.
Fig. 9. Magnetic conﬁgurations and contributions to the linear dichroism in the LSMO/BTO system at room temperature (a, b),
and at elevated temperatures (c, d). The LSMO/LSAT sample at room temperature is shown (e) for comparison.
Thus with such a strong elastic coupling between ﬁlm and substrate and the ability to dynamically tune the strain state of the ﬁlm with reorientation of the BTO ferroelec-tric axis, we show that this model artiﬁcial multiferroic can hold promise for room-temperature magneto-electric coupling at the nanoscale, and furthermore shows a possi-ble materials system to be employed in sub-micron devices that exploit electric ﬁeld control of magnetic anisotropy.
The authors would like to thank C.W. Schneider for the use of his X-ray diﬀractometer, and L. Le Guyader and M. Buzzi for assistance with image analysis software. Part of this work was performed at the Swiss Light Source, Paul Scherrer Insti-tute, Villigen, Switzerland. The Advanced Light Source is sup-ported by the Director, Oﬃce of Science, Oﬃce of Basic Energy Sciences, of the U.S. Department of Energy under Contract No. DE-AC02-05CH11231. This work was partially funded by EU’s 7th Framework Program IFOX (NMP3-LA-2010 246102).
1. C.A.F. Vaz, J. Hoﬀman, C.H. Ahn, R. Ramesh, Adv. Mater. 22, 2900 (2010)
2. R. Datta, S. Kanuri, S.V. Karthik, D. Mazumdar, J.X. Ma, A. Gupta, Appl. Phys. Lett. 97, 071907 (2010)
3. F. Tsui, M.C. Smoak, T.K. Nath, C.B. Eom, Appl. Phys. Lett. 76, 2421 (2000)
4. M.K. Lee, T.K. Nath, C.B. Eom, M.C. Smoak, F. Tsui, Appl. Phys. Lett. 77, 3547 (2000)
5. D. Dale, A. Fleet, J.D. Brock, Y. Suzuki, Appl. Phys. Lett.
82, 3725 (2003)
6. W. Eerenstein, M. Wiora, J.L. Prieto, J.F. Scott, N.D. Mathur, Nat. Mater. 6, 348 (2007)
7. R.V. Chopdekar et al., Phys. Rev. B 86, 014408 (2012) 8. A. Tebano et al., Phys. Rev. Lett. 100, 137401 (2008) 9. M. Huijben, L.W. Martin, Y.H. Chu, M.B. Holcomb,
P. Yu, G. Rijnders, D.H.A. Blank, R. Ramesh, Phys. Rev. B 78, 094413 (2008)
10. C. Aruta, G. Ghiringhelli, V. Bisogni, L. Braicovich, N.B. Brookes, A. Tebano, G. Balestrino, Phys. Rev. B 80, 014431 (2009)
11. R.V. Chopdekar, E. Arenholz, Y. Suzuki, Phys. Rev. B 79, 104417 (2009)
12. U. Flechsig, F. Nolting, A.F. Rodriguez, J. Krempasky, C. Quitmann, T. Schmidt, S. Spielmann, D. Zimoch, Am. Inst. Phys. Confer. Proc. 1234, 319 (2010)
13. C. Piamonteze et al., J. Synchr. Rad. 19, 661 (2012) 14. J. St¨ohr, H.A. Padmore, S. Anders, T. Stammler, M.R.
Scheinfein, Surf. Rev. Lett. 5, 1297 (1998)
15. C.A.F. Vaz, J. Hoﬀman, Y. Segal, M.S.J. Marshall, J.W. Reiner, Z. Zhang, R.D. Grober, F.J. Walker, C.H. Ahn, J. Appl. Phys. 109, 07D905 (2011)